### Statistics

### Views

- Total Views
- 1,610
- Views on SlideShare
- 1,317
- Embed Views

### Actions

- Likes
- 0
- Downloads
- 0
- Comments
- 0

Like this document? Why not share!

- Principles of corrosion by Prof. TKG Nambood... 9784 views
- TALAT Lecture 5102: Reactivity of t... by CORE-Materials 1877 views
- Electrochemical measurements of ano... by iaeme 431 views
- Corrosion and prevention basic prin... by Prof. TKG Nambood... 9327 views
- What are batteries, fuel cells, and... by Jupira Silva 981 views
- Sustainable hydrogen and electrical... by TU Delft OpenCour... 550 views
- Corrosion inhibition Effect of Cety... by Dr Arwind Kumar D... 340 views
- Corrosion Inhibition Effect of Brij... by Dr Arwind Kumar D... 357 views
- Corrosion Inhibition Effect of Poly... by Dr Arwind Kumar D... 461 views
- TALAT Lecture 5103: Corrosion Contr... by CORE-Materials 4281 views
- Corrosion Control Casti by Charlie Chong 16577 views
- Science of corrosion by Narayana Reddy Pa... 3654 views

**1,610**views

- Total Views
- 1,610
- Views on SlideShare
- 1,317
- Embed Views
- 293

- Likes
- 0
- Downloads
- 0
- Comments
- 0

http://ocw.tudelft.nl | 293 |

- Chapter 3KINETICS OFACTIVATIONPOLARIZATION3.1 INTRODUCTIONElectrochemical reaction kinetics is essential in determining the rate ofcorrosionof a metal M exposed to a corrosive medium (electrolyte). On the other hand,thermodynamics predicts the possibility of corrosion, but it does not provideinformation on how slow or fast corrosion occurs. The kinetics of a reactionon a electrode surface depends on the electrode potential. Thus, a reactionrate strongly depends on the rate of electron flow to or from a metal-electrolyteinterface. If the electrochemical system (electrode and electrolyte) is at equi-librium, then the net rate of reaction is zero. In comparison, reaction rates aregoverned by chemical kinetics, while corrosion rates are primarily governed byelectrochemical kinetics.Electrochemical kinetics of a corroding metal can be characterized by deter-mining at least three polarization parameters, such as corrosion current densitycorrosion potential and Tafel slopes and/or Thenthe corrosion behavior can be disclosed by a polarization curve (E vs.Evaluation of these parameters leads to the determination of the polarizationresistance and the corrosion rate as which is often converted intoFaradaic corrosion rate having units of This is an acceleratedelectrochemical process for determining that has an advantage over thedetermined by weight loss since the latter is a time consuming process, whichmay lead to unsatisfactory results when changes with time [13]. Instead,a polarization curve is readily obtained and it can offer a practical method forcharacterizing electrochemical kinetics parameters.
- 72 CHAPTER 3. KINETICS OF ACTIVATION POLARIZATION3.2 ENERGY DISTRIBUTIONFor a polarized electrode under steady-state current flow, the generalized re-action given by eq. (1.2) can be used to derive the Butler-Volmer equation,which involves energy barriers known as activation energies. Only the activa-tion energy change is used for the forward (reduction) and reverse(oxidation) reactions. For example, the hydrogen reaction, atequilibrium requires that the rate of discharge of in the forward direc-tion (reduction) must be exactly equal to the rate of ionization of moleculein the reverse direction (oxidation). However, if deviation from the equilibriumstate occurs, an overpotential develops and consequently, the electrochemicalcell polarizes and the activation energies become dependent on the exchangecurrent density These energies are depicted in Figure 3.1 in which theactivation state is at the maximum point (saddle point). This figure rep-resents the Boltzmann or Maxwell-Boltzmann distribution law for the energydistribution of the reacting species (ions) [4,7]. This schematic energy distribu-tion is for reversible electrodes. If these are polarized by an overpotential understeady-state conditions, the rate of reactions are not equal,
- 3.2. ENERGY DISTRIBUTION 73In general, the electrochemical and chemical rates of reactions due to eitheranodic or cathodic overpotentials can be predicted using both Faraday andArrhenius equations, respectivelywhere = Applied current density= Atomic weight of speciesin units of= Oxidation state or valence number= Valence number of element= Weight fraction of element= Chemical reaction constant= Activation energy or free energy change (J / mol)At equilibrium, Faraday’s and Arrhenius’ rate equations become equaland consequently, the current density becomesHere, the term may be defined as the electrochemical rateconstant having unit of current density For a reversible electrodeat equilibrium, the current density in eq. (3.3) becomes the exchange currentdensity; that is, In addition, Table 3.1 gives typical experimental valuesfor
- 74 CHAPTER 3. KINETICS OF ACTIVATION POLARIZATIONOn the other hand, if an electrode is polarized by an overpotential understeady-state conditions, then the rates of reactions are not equaland consequently, the forward (cathodic) and reverse (anodic) current densitycomponents must be defined in terms of the free energy change deducedfrom Figure 3.1. Hence,where= Symmetry coefficientFor a cathodic case, the net current and the overpotential are andrespectively. Substituting eqs. (3.4) and (3.5) into this expression yields thenet current density in a general formfrom which the exchange current density is deduced asSubstituting eq. (3.7) into (3.6) for one-step reaction yields the well-knownButler-Volmer equation for polarizing an electrode from the open-circuitpotential under steady-state conditionswhereE = Applied potentialIt is clear that overpotential depends on the applied current density; there-fore, In addition, the exchange current density can be definedas the rate of oxidation and reduction reactions at equilibrium. Specifically,is the current density at which the rate of oxidation and rate of reductionare equal in a state of equilibrium. Thus, is just the reversible reaction rateat equilibrium and it is a kinetic parameter, whereas is a thermodynamicparameter.
- 3.2. ENERGY DISTRIBUTION 75In fact, is very sensitive toelectrode surface condition and it is temperature-dependent as indicated by eq. (3.8). Thus, one can generalize the Arrheniusequation, eq. (3.2), for a series of electrochemical reactions as follows [47]where = Exchange current density at temperature T= Reference exchange current density at temperature= 1,2,3,4,... = Number of reactions.This expression, eq. (3.8), is the general non-linear rate equation in termsof current density that most electrochemical cells obey under charge-transfercontrol. Thus, and are theanodic and cathodic overpotentials, respectively, which represent a deviationfrom the half-cell potential and E is the applied potential. In summary,the applied anodic current density is and the cathodiccurrent density is At equilibrium conditions, the potentialis and eq. (3.8) yields This implies thatthe rates of metal dissolution (oxidation) and deposition (reduction) are equal.However, a deviation from equilibrium of the half-cells is the normal casein real situations.Furthermore, if one is interested in determining the total ionic molar fluxJdue to the mass transfer of a species then andThis ionic molar flux will be defined in details in Chapter 4. The reactionrate in terms of current density given by eq. (3.8) is valid for one-step reaction.Hence, the controlling reaction may be part of a series of reaction steps, but theslowest reaction step is the rate-controlling. For any reaction, eq. (3.8) can beapproximated by letting and Expandingthe exponential functions according to Taylor’s series yieldsThus, eq. (3.8) can be expressed as a linear approximation when the over-potential is small in magnitudeand
- 76 CHAPTER 3. KINETICS OF ACTIVATION POLARIZATIONEq. (3.13) and (3.14) can be used for small values of overpotential like[7]. However, one can take a different approach to approximate thecurrent density by considering the following inequalityIf this is the case, then eq. (3.8) yieldSolving eq. (3.16) for the overpotential yields the Tafel equationwhereIn fact, eq. (3.17) yields a linear behavior when for either ananodic polarization or cathodic polarization analysis. With regard to reactionrates, let and be the forward (reduction) and reverse (oxidation) reactionrates, respectively and let be the equilibrium constant. Thus,and from eq. (3.2),Substituting eqs. (b) and (c) into (a) yieldsDifferentiating eq. (d) with respect to the temperature T givesRearranging eq. (f) yields the activation energy [5]
- 3.2. ENERGY DISTRIBUTION 77In addition, Faraday’s law of electrolysis describes the quantitative relation-ship for determining the rate of charge transfer in terms of current. Thus, thequantity of charge transferred (Q) at a time is Q = It, and the quantity ofmoles for zF charge transfer is Now, the Faraday’s weight loss orgain can be deduced by multiplying the number of moles, eq. (3.12b), by theatomic weight of metal MExample 3.1 Two identical zinc rods are exposed to HCl-base electrolyte.One rod is immersed at 25°C for 2 hours, while the other rod is at 50°C for1 hour. Calculate the time of exposure of a third identical rod immersed theelectrolyte at 30 °C.Solution:The zinc oxidation reaction is which requires an chem-ical activation energy to proceed in the written direction. The zinc rods are notpolarized through an external circuit. Thus, the Arrhenius equation, eq. (3.2),yieldsDividing these equations givesThen, at and withand at and the reaction rates areThen, the activation energy becomes
- 78 CHAPTER 3. KINETICS OF ACTIVATION POLARIZATIONSubstituting this energy into eq. and solving for yields@, the time and rate of reaction are, respectivelyFor comparison purposes, the reaction rates areExample 3.2 Given the following data for a hypothetical metal undergoingchemical oxidation in a aqueous solution, a) plot the data (Arrhenius plot) anddetermine the activation energy from the plot and b) calculate the chemical rateat 308°C.Solution:a) Using eq. (3.2) to curve fit the given data yields the resultant curve fittingequation
- 3.2. ENERGY DISTRIBUTION 79where and the Therequired Arrhenius plot is shown below.Example 3.3 Determine the atomic weight of alloy.Solution:The state of oxidation and the atomic weight of each element areThe atomic weight of the alloy isb) If T = 308K, then and
- 80 CHAPTER 3. KINETICS OF ACTIVATION POLARIZATION3.3 POLARIZATIONThis section partially treats the copious literature for supporting the mathemat-ical models for characterizing the kinetics ofcharge transfer mechanism involvedin an electrochemical system. Thus, electrode reactions are assumed to inducedeviations from equilibrium due to the passage of an electrical current throughan electrochemical cell causing a change in the working electrode (WE) poten-tial. This electrochemical phenomenon is referred to as polarization. In thisprocess, the deviation from equilibrium causes an electrical potential differencebetween the polarized and the equilibrium (unpolarized) electrode potentialknown as overpotential [1].Figure 3.2 shows a partial polarization diagram and related kinetic parame-ters. For instance, both Evans and Stern diagrams are superimposed in orderfor the reader to understand the significance of the electrochemical behavior ofa polarized metal (M) electrode in a hydrogen-containing electrolyte.From Figure 3.2, and are the open-circuit potentials for hydrogenand metal M, respectively, are the exchange current densities, andis the limiting current density.For a reversible electrode, Evans diagram allows the determination of thecorrosion point where both the hydrogen cathodic and the metal anodic lineintercept. On the other hand, the irreversible electrochemical behavior denotedby the cathodic and anodic Stern diagram is also used for determining the cor-rosion point by simply extrapolating the linear portions of both curves until the
- 3.4. ACTIVATION POLARIZATION 81intercept as indicated in Figure 3.2. The latter diagram is a very common inelectrochemical studies of pure metals and their alloys. Therefore, both Evansand Stern polarization diagrams provide the corrosion potential and thecorrosion current density The other parameters illustrated in Figure 3.2will become relevant as the electrochemical analysis advances in this chapter.With respect to the Stern diagram, this represents a polarization behavior thatcan be determined experimentally using potentiostatic and potentiodynamicmethods, and it will be referred to as a polarization curve. Thus, a polariza-tion curve is the result of polarizing from the corrosion potential anodically orcathodically and it is a very common experimental output in electrochemicalstudies on corroding electrodes.Evaluation of corrosion behavior is normally done through a function thatdepends on kinetic parameters depictedinFigure 3.2. Hence, the current densityfunction for polarizing an electrode irreversibly from the corrosion potential issimilar to eq. (3.8). Hence,whereE = Applied potential (V)= Anodic polarization constant (Tafel anodic slope) (V)= Cathodic polarization constant (Tafel cathodic slope) (V)Moreover, anodic polarization caused by ananodicoverpotentialis referred to as an electrochemical process in which a metal surface oxidizes(corrodes) by losing electrons. Consequently, the metal surface is positivelycharged due to the loss of electrons. This electrochemical polarization is quanti-fied by On the other hand, cathodic polarization requires that electrons besupplied to the metal surface at an negative overpotential,which implies that3.4 ACTIVATION POLARIZATIONIn general, the activation polarization is basically an electrochemical phenom-enon related to a charge-transfer mechanism, in which a particular reactionstep controls the rate of electron flow from a metal surface undergoing oxida-tion. This is the case in which the rate of electron flow is controlled by theslowest step in the half-cell reactions [1-4].Despite that eq. (3.22) is a generalized expression, it represents a measureof anodic polarization for corrosion studies and indicates that for anunpolarized and for a polarized electrode surface. For the latter case,the reaction rate for activation polarization depends on the charge-transfer over-potential as in metal oxidation due to electrons loss, the diffusion overpotentialas in mass transport of ions, the reaction overpotential due to rate determin-ing chemical reaction mechanism, the crystallization overpotential as in metal
- 82 CHAPTER 3. KINETICS OF ACTIVATION POLARIZATIONdeposition in which atoms are incorporated into the electrode crystal surface lat-tice, and the Ohmic overpotential due to a resistance at the electrode/terminaljunctions[2].In general, the anodic metal undergoes a succession of reaction steps priorto dissolve in the electrolyte. This succession is hypothetically shown by thefollowing idealized metal oxidation reactions during activation polarizationThis succession indicates that the metal M looses electrons on its surfaceand eventually the metal cation goes into solution. If the metal is silverundergoing oxidation, then the cation is just For iron, the succession maybeFor hydrogen evolution, Fontana’s idealized model [1] for activation polar-ization is depicted in Figure 3.3 can be used to explain the succession of thereaction steps that may take place after the hydrogen cations are adsorbed (at-tached) on the electrode surface. Hence, the possible reaction steps areThus, only one step in eq. (3.23) and one in eq. (3.24) controls the chargetransfer for activation polarization. For instance, the formation of hydrogengas bubbles on the metal electrode surface is the last step in the successionof reactions and eventually, the bubbles move to the surface of the electrolytewhere they burst.
- 3.5. POLARIZATION METHODS 83According to the model in Figure 3.3, the metal oxidation process can berepresented by the following redox stoichiometric reactionOn the other hand, if this reaction is reversed, then the metalcations in solution, specifically at the electrode/electrolyte interface, aredeposited (plated) on the metal electrode. This is possible since electrons in thesolution are supplied to the electrode surface. Thus, cathodic polarization oc-curs giving a negative overpotential, In any event, anodic and cathodicreaction rates are assumed to be sufficiently slow.3.5 POLARIZATION METHODSThe polarization resistance of a metal/electrolyte system and the pitting orbreakdown potential can be determined using at least two-electrode system.Subsequently, the rate of metal dissolution or corrosion rate is calculated usinga function of the form The methods areLinear Polarization (LP) as schematically shown in Figure 3.4 covers bothanodic and cathodic portions of the potential E versus current densitycurvefordeterminingTafel Extrapolation technique (TE) (Figure 3.2) takes into account thelinear parts of the anodic and cathodic curves for determiningElectrochemical Impedance Spectroscopy (EIS) as schematically shownin Figure 3.10 requires an alternating current (AC) and the output is aNyquist plot for charge-transfer or diffusion control process, which canbe used to determine which in turn, is inversely proportional to thecorrosion current densityStandard or recommended experimental procedures for measurements ofcan be found in the American Society for Testing Materials ASTM G-59 andASTM G-106 testing methods, and ASTM G-5 is for anodic potentiodynamicstudies, are included in the annual Book of ASTM Standards Vol. 03.02.3.5.1 LINEAR POLARIZATIONFirst of all, using eq. (3.8) under anodic and cathodic polarization individually,the Tafel slopes are derived by letting for ananodic polarization analysis,where On the other hand,is for characterizing cathodic polarizationwhen Under these conditions, eq. (3.8) reduces to
- 84 CHAPTER 3. KINETICS OF ACTIVATION POLARIZATIONSolving eqs. (3.25) for the overpotential yieldswhere and are known as Tafel slopes of the anodic and cathodic reac-tions, respectively. These slopes are defined byAdditionally, if then Figure 3.4 shows a theoreticalpolarization curve for conducting polarization resistance measurements.
- 3.5. POLARIZATION METHODS 85The linear polarization is confined to a small magnitude of the overpotentialsand respectively, using linear coordinates. This technique allows thedetermination of using a potential range of ±10 mV from the [3].Prior to determining the polarization resistance is estimated from thelinear slope of the curve (Figure 3.4) asThe corresponding corrosion current density depends on kinetic parameterssince Thus, the simple linear relation that defines the corrosioncurrent density is of the formwhere and and are taken as positive kinetic parame-ters for determining of a corroding or oxidizing metallic material. Noticethat eq. (3.29) predicts that the corrosion current density is very sensitive tochanges in the polarization resistance. In fact, the magnitude of the polarizationresistance is mainly controlled by the corrosion current density [1,46]. Hence,This constant will be derived in the next section. In fact, this methodrequires knowledge of the Tafel anodic and cathodic slopes in order tocalculate and subsequently predict using eq. (3.29). This expressionis simple, but essential in corrosion measurements since can be convertedto corrosion rate in units of which are more convenient for engineeringpurposes after and are determined. finally, the values of these slopes areand and3.5.2 TAFEL EXTRAPOLATIONThis method involves the determination of the Tafel slopes and as wellas and from a single polarization curve as shown in Figure 3.2.This curve is known as the Stern diagram (non-linear polarization) based on eq.(3.22). The Evans diagram (linear polarization) is also included in order to showthat both diagrams have a common point. This figure illustrates ahypothetical electrochemical behavior of a metal M immersed in an electrolytecontaining one type of oxidizer, such as ions.For electrochemical systems containing several oxidizers, determining thecorrosion point is more complex using the Evans diagram, but the Stern dia-gram would provided a similar polarization curve as shown in Figure 3.2, fromwhich both and are easily determined by extrapolating the Tafelanodic and cathodic linear parts until they intersect as straight lines. Also in-cluded in Figure 3.2 are the exchange current densities, and and their
- 86 CHAPTER 3. KINETICS OF ACTIVATION POLARIZATIONcounterpart potentials, and forhydrogenevolutionandmetaloxida-tion, respectively. These potentials, and are known as open-circuitpotentials. Furthermore,the limiting current density for cathodic polariza-tion is included as an additional information one can extract from a cathodicpolarization curve. The latter term will be dealt with in Chapter 5.Further analysis of Figure 3.2 yields the following summary:The solid curve can be obtained statically or dynamically.This non-linear curve is divided into two parts. If the uppercurve represents an anodic polarization behavior for oxidation of the metalM. On the contrary, if the lower curve is a cathodic polariza-tion for hydrogen reduction as molecular gas (hydrogen evolution). Bothpolarization cases deviate from the electrochemical equilibrium potentialdue to the generation of anodic and cathodic overpotentials, whichare arbitrarily shown in Figure 3.2 as and respectively.Both anodic and cathodic polarization curves exhibit small linear partsknown as Tafel lines, which are used for determining the Tafel slopesand These slopes can be determined using either the Evans or Sterndiagram.Extrapolating the Tafel or Evans straight lines until they intersect definethe point.The disadvantage in using the Evans diagram is that the exchange currentdensity the open-circuit potential (no external circuit is applied),and the Tafel slopes for the metal and hydrogen have to be known quan-tities prior to determining the point.The advantage of the Stern diagram over the Evans diagram is that it caneasily be obtained using the potentiodynamic polarization technique at aconstant potential sweep (scan rate) and no prior knowledge of the abovekinetics parameter is necessary for determining the point. Theresultant curve is known as a potentiodynamic polarization curve.Inconclusion, and can be determined from an Evans diagramfor an unpolarized metal since at Onthe other hand, if the metal is polarized, then the Stern diagram canbe used for determining and In addition, is areversible potential also known as a mixed potential. Further analysis ofthe polarization phenomenon requires use of the Ohm’s law. Hence, thecell and the inner potentials are defined by, respectively
- 3.5. POLARIZATION METHODS 87where I = Current (A)= External resistance (Ohm = V / A)= Solution resistance (Ohm = V / A)= Internal potential (V)Solving eq. (3.31) for I yieldsThe current in eq. (3.33) strongly depends on the magnitude of the externalresistance. A slight decrease in increases the current I. Hence, ifthen and when In addition, asWith regard to eq. (3.32), can be neglected due to its small contributionto the cell potential. However, the electrolyte conductivity is of significance indetermining the governing current expression. For instance, whenthe electrolyte has a high conductivity and if the electrolyte has alow conductivity. Hence, from eq. (3.33) the governing current expressions areNowadays, sophisticated instrumentation, such as a potentiostat/galvanostatis commercially available for conducting electrochemical experiments for char-acterizing the electrochemical behavior a metal or an alloy in a few minutes.Nevertheless, a polarization diagram or curve is a potential control technique.This curve can experimentally be obtained statically or dynamically. The lat-ter approach requires a linear potential scan rate to be applied over a desiredpotential range in order to measure the current response.On the other hand, a galvanostat can be used as the current control sourcefor determining the potential response on a electrode surface. However, the po-tential control approach is common for characterizing electrochemical behaviorof metallic materials. The potential can be applied uniformly or in a stepwisemanner using a waveform. The former case generates a steady-state currentresponse, while the latter provides a transient current response.Further interpretation of the polarization curves can be extended using Pour-baix graphical work depicted in Figure 3.5 for pure iron (Fe). The resultantplots represent the functions and for an electrolyte con-taining atAdditionally, the reactions depicted in Figure 3.5 and some related kinetic pa-rameters are listed in Table 3.2 for convenience. One important observation isthat both anodic and cathodic Tafel slopes, and respectively are equal nu-merically and consequently, Figure 3.5b has an inflection point atThis electrochemical situation is mathematically predicted and discussed in thenext section using a current density function for a mixed-potential system.
- In fact, Figure 3.5 compares both linear and extrapolation results for iron.The interpretation of this figure is based on complete activation control in theabsence of diffusion and external current [46]. Thus, it can be deduced fromthis figure thatthe net current density is zero at equilibrium, but the cor-rosion current density is at the corrosion potential,The polarization curves are reversible in nature; however, if irreversibilityoccurs, the heavy line in Figure 3.5a would follow the vertical axis at apotential range whenThe open-circuit potentials, and can be estimated using theNernst equation.One important fact is that the solution must be continuously stirred to keepa uniform concentration of the species in solution; otherwise, the concentration88 CHAPTER 3. KINETICS OF ACTIVATION POLARIZATION
- 3.5. POLARIZATION METHODS 89at the electrodes become uneven and the open-circuit potential increasesduring oxidation and decreases during reduction. At equilibrium, theoverpotential becomes since the applied potential and theapplied current density are and respectively. However, ifthe iron reaction is irreversible because it corrodes by liberating electrons.Combining the Pourbaix diagram and the polarization curves for iron inwater at yields interesting information on the electrochemical state asshown in Figure 3.6, which includes the hydrogen and oxygen lines for com-parison [46]. Observe the correspondence of potential between both diagrams.For instance, the potential at point A, indicates that corrosion occurs along lineCP, but at point B the potential suggests that passivation occurs and iron isprotected anodically. Point P is a transitional potential at the critical currentdensity. Any slight change in potential iron passivates at or corrodesat Also, If Pourbaix predicts immunity, but the polarizationcurve indicates that corrosion is possible.Furthermore, the advantage of the Pourbaix diagram as shown in Figure3.6a is that it predicts the electrochemical state for immunity, corrosion, andpassivation, and it is related to the polarization curve shown in Figure 3.6b.However, only the polarization curve predicts the corrosion rate through thecurrent density for metal oxidation and the passivation rate through thepassive current density for metallic cation reduction to form an oxide protectivefilm on the electrode surface. The passivation phenomenon is discussed in detailsin Chapter 6.
- 90 CHAPTER 3. KINETICS OF ACTIVATION POLARIZATION3.6 CORROSION RATEDuring corrosion (oxidation) process, both anodic and cathodic reaction ratesare coupled together on the electrode surface at a specific current density knownas This is an electrochemical phenomenon which dictates that both re-actions must occur on different sites on the metal/electrolyte interface. For auniform process under steady state conditions, the current densities at equilib-rium are related as Assume that corrosion is uniformand there is no oxide film deposited on the metal electrode surface; otherwise,complications would arise making matters very complex. The objective at thispoint is to determine both and either using the Tafel Extrapolationor Linear Polarization techniques. It is important to point out that can-not be measured at since and current will not flow through anexternal current-measuring device [3].When polarizing from the corrosion potential with respect to anodic or ca-thodic current density, the overpotential expressions given by eqs. (3.26a) and(3.26b)becomeRecall that andnow represent the potential changes from the steady-state corrosion potentialSolving eqs. (3.35a) and (3.35b) for the anodic and cathodic currentdensities yields, respectivelyAssuming that the applied current density is and substitutingeqs. (3.36) and (3.37) into this expression yields the Butler-Volmer equationthat quantifies the kinetics of the electrochemical corrosionThis expression resembles eq. (3.22), but it is a convenient expression at thispoint since the inverse polarization resistance is easily obtainable by derivingeq. (3.38) with respect to the applied potential E. Thus,
- 3.6. CORROSION RATE 91Further,Let’s set some conditions for eq. (3.40) such thatEvaluating eq. (3.40) at the inflation point yieldswhich clearly indicates that the inflection point is achieved if and only ifThis condition was pointed out by Oldham and Mansfield [13] as themathematical proof for the point depicted in Figure 3.2.Additionally, evaluating eq. (3.39) at yields the polarizationresistanceThus,Here, is the proportionality constant defined by (3.30). Notice that isinversely proportional to as indicated by eq. (3.45) and depicted in Figure3.7a, but it can be linearized as shown in Figure 3.7b. Thus,In general, a corroding metal is equivalent to a short-circuit cell or energy-producing system, in which energy dissipation occurs during the production ofa corrosion product [3].
- 92 CHAPTER 3. KINETICS OF ACTIVATION POLARIZATIONThus, metal oxidation is equivalent to metal corrosion. Now, dividing Fara-day’s rate of reaction, eq. (3.1), by the metal density defines the corrosionrate (rate of metal dissolution) asIn addition, corrosion rate can be represent by the rate of weight loss [1]or rate of penetration [4], but eq. (3.48) is a mathematical model convenientfor determining the metal dissolution in terms penetration per year in units ofThese are common units to the engineers or designers.Example 3.4 Calculate the corrosion rate in units of andthe electrochemical rate constant in and for a low carbonsteel plate immersed in sea water. Given data:(current), andSolution:Since the carbon steel is basically iron (Fe), the oxidation reaction involvedin this problem is with and F = 96,500and the exposed area is Then, the current density isUsing eq. (3.48), the corrosion rate is
- 3.6. CORROSION RATE 93From eq. (3.1), the electrochemical rate constant isEliminating the atomic weight in eq. (3.1) yieldsExample 3.5 Assume that the rates of oxidation of and reduction ofare controlled by activation polarization. Use the data given below to a)plot the appropriate polarization curves and determine and from theplot. Calculate b) both and c) the corrosion rate in andthe polarization resistance in Data:Solution:a) E vs. plot1) Plotand2) Draw the hydrogen reduction and zinc oxidation lines with andslopes, respectively3) The intercepting point defines the corrosion point asfor the unpolarized metal. In addition,at and and are the open-circuit potentials, which canbe determined using the Nernst equation, eq. (2.32).
- 94 CHAPTER 3. KINETICS OF ACTIVATION POLARIZATIONb) Using eqs. (3.26a) and (3.26b) with andyieldsEquating eqs. (c) and (d) and solving for yields the corrosion currentdensityLetting and using eg. (a) or (b) givesc) From eg. (3.48)d) From eq. (3.30),
- 3.6. CORROSION RATE 95and from eq. (3.45),Example 3.6 A copper surface area, is exposed to an acidsolution. After 24 hours, the loss of copper due to corrosion (oxidation) isCalculate a) the current density in b) the corrosionrate in and c) the number of reactions per unit time. Use the data:Solution:First of all, the corrosion process of copper can be represented by the followinganodic reaction:where the valence is Z = +2. Thus,a) According to Faraday’s law the current density isb) From eq. (3.48),
- 96 CHAPTER 3. KINETICS OF ACTIVATION POLARIZATIONc) Recall that 1 C = so that Thus,the number of reactions per time in seconds isExample 3.7 An electrochemical cell shown below was used as a concen-tration cell in order to measure the current due to the difference in ionic con-centration between the anodic half-cell and the cathodic-half cell. Determinethe corrosion rate in terms of electrons/second and the number of anodic reac-tions/second if the measured current isSolution:The oxidation of copper (corrosion) is due to the following anodic reaction:and the reduction of copper (electroplating) is due to cathodic reaction
- 3.7. IMPEDANCE SPECTROSCOPY 97Clearly, the oxidation state is Z = 2. Thus, the corrosion rates areAlso,3.7 IMPEDANCE SPECTROSCOPYThe electrochemical impedance spectroscopy (EIS) method is very useful incharacterizing an electrode corrosion behavior. The electrode characteriza-tion includes the determination of the polarization resistance corrosionrate and electrochemical mechanism [1,4,6,19-28]. The usefulness of thismethod permits the analysis of the alternating current (AC) impedance data,which is based on modeling a corrosion process by an electrical circuit. Severalreview papers address the electrochemical impedance technique based on theAC circuit theory [22-24,29-30].The EIS technique is based on a transient response of an equivalent circuit foran electrode/solution interface. The response can be analyzed by transfer func-tions due to an applied small-amplitude potential excitation at varying signalsor sweep rates. In turn, the potential excitation yields current response and viceverse. In impedance methods, a sine-wave perturbation of small amplitude isemployed on a corroding system being modeled as an equivalent circuit (Figure3.8) for determining the corrosion mechanism and the polarization resistance.Thus, a complex transfer function takes the formThe transfer functions depend on the angular frequency and are expressed asimpedance and admittance It should be emphasized that isthe frequency-dependent proportionality factor of the transfer function betweenthe potential excitation and the current response. Thus, for a sinusoidal current
- 98 CHAPTER 3. KINETICS OF ACTIVATION POLARIZATIONperturbation, the transfer function is the system impedance and for asinusoidal potential perturbation, the transfer function is the system admittanceHence,where = Time-dependent potential (V)= Time-dependent current (A)= Angular frequency= Real parts= Imaginary parts= Time (s)= Imaginary operatorIn addition, Ohm’s law can be viewed in two different current impositioncases as per ASTM G-106 standard testing method. Hence,Here, is the magnitude of the impedance containing elements of anequivalent circuit, such as capacitors and inductors. Capacitors oppose or im-pede the current flow. In modeling an electrochemical system as an electro-chemical circuit, a potential waveform is applied across the circuit and a cur-rent response to the frequency signal generates impedance data. Thus, theimpedance data is related to a phase shift angle and a variation in potential andcurrent amplitudes. This technique is a straightforward approach for analyzingthe corrosion behavior of a metal [24]. Figure 3.8 shows two schematic electro-chemical circuit models. For a charge-transfer control (Figure 3.8a), only thesolution resistance polarization resistance and the capacitorare needed in a simple circuit. On the other hand, if the electrochemical systemis diffusion-control (Figure 3.8b), a diffusion impedance is incorporated inthe circuit.= Signal frequency
- 3.7. IMPEDANCE SPECTROSCOPY 99The potential excitation and its current response are schematically shownin Figure 3.9 as sinusoidal excitations. The electrochemical impedance spec-troscopy method is conducted according to the ASTM G-106 standard practice,in which a range of small-amplitude sinusoidal potential perturbation is appliedto the electrode/solution interface at discrete frequencies. These frequenciescause an out of phase current response with respect to the applied sinusoidalpotentialwaveform.If a sinusoidal potential excitation is applied to the electrode/solution inter-face, the potential, current and impedance can be predicted as per Barn andFaulkner mathematical models [6]. Thus,where = Constants= Phase shift angle between andand (intermediate)
- 100 CHAPTER 3. KINETICS OF ACTIVATION POLARIZATIONThe magnitude of and areand the phase shift angle is defined asThe fundamental characteristic of an AC signal in a simple electrochemicalcircuit (Figure 3.8a) is described by the impedance of the form [22,24]where C is the interfacial capacitance of a electrical double-layer at theelectrode surfaceFor low and high frequency amplitudes, eq. (3.59) yieldsCombining eqs. (3.60) and (3.61) yields the polarization resistance aswhich is the sought output in electrochemical impedance measurements.Equating eqs. (3.45a) and (3.62) yields the corrosion current density in termsof impedanceUpon using Faraday’s law, eq. (3.63) becomesFurther analysis of eq. (3.59), together with eq. (3.52), yields the impedanceequation of a circle [22]. Hence,
- 3.7. IMPEDANCE SPECTROSCOPY 101andThen, the equation of a circle for charge-control mechanism becomes [22]The locus of eq. (3.68) is schematically shown in Figure 3.10 with a radiusof This figure is known as the Nyquist plot, from which the maximumphase shift angle and polarization resistance becomeFigure 3.11 shows Nyquist plots of a AISI 1030 steel immersed in phosphoricacid containing butanol and thiosemicarbonate (TSC) at room tem-perature. These data is for a charge-control mechanism with and without the
- 102 CHAPTER 3. KINETICS OF ACTIVATION POLARIZATIONTSC inhibitor [26]. Notice from this Figure 3.11 that the Nyquist impedancesemicircles increase with increasing content of the TSC inhibitor. This impliesthat the polarization resistance also increases with additions of this in-hibitor, which in turn, decreases the corrosion rate as indicated in Table3.3.In addition, the double-layer capacitance can be calculated using thefollowingexpression [31]Table 3.3 gives relevant experimental data extracted from the complex Nyquistplot elucidated in Figure 3.11.On the other hand, Figure 3.12 shows schematic Bode plots for the circuitin Figure 3.8a with three polarization resistance values. This type of plots showthe effect of angular frequency on the impedance and phase shift angle.
- 3.7. IMPEDANCE SPECTROSCOPY 103When an electrochemical process is controlled by diffusion orfilmadsorption,the electrochemical system can be modeled using the ideal circuit shown inFigure 3.8b. In this case, a diffusion impedance is included in the circuitseries and it is known as Warburg impedance. Notice that and areconnected in series. An ideal Nyquist-Warburg plot is shown in Figure 3.13
- 104 CHAPTER 3. KINETICS OF ACTIVATION POLARIZATIONThe interpretation of Figure 3.13 indicates that the 45° portion of the linecorresponds to a low angular frequency range. In this case, the kinetics of theelectrochemical system is limited by a diffusion-control process (concentrationpolarization). Also, extrapolating the semicircle (dashed curve) to intercept thereal impedance axis graphically defines the polarization resistanceA particular case for using is when diffusion through a surface film is therate-controlling of carbon steel immersed in concentrated sulfuric acidThus, iron (Fe) oxidizes and forms a film [25].Figure 3.14 shows an experimental Nyquist-Warburg plot for a precipitationhardening (aged) 2195 Al-Li alloy. Notice that the semicircle is depressed dueto a diffusion process, which is confirmed by the 45° line. The polarizationresistance for this alloy is in an aerated solution containing 3.5%NaCl at 21.5°C.The diffusion impedance expression due the formation of a thin oxide film isdefine by [31-32]where = Warburg impedance coefficient =Thickness of the diffusion layer, =Concentration of the specie in the diffusionlayer and A = Exposed area.For the 45° Warburg line in Figure 3.13, becomes
- 3.8. CHARACTERIZATION OF ELECTROLYTES 105since and from whichFurthermore, the impedance of a depressed Nyquist plot due to surfaceroughness, dielectric inhomogeneities and diffusion is defined as the Cole-Coleimpedance formula [33-36]. Hence,3.8 CHARACTERIZATION OF ELECTROLYTESAssume that an electrolyte solution contains positively and negatively chargedions (particles) with valence equals to and respectively. If the solutionhas different type of ions, the number of cations and anions are,respectivelywhere = Represents species or ions of different valance= Number of molesLet an applied electrical field disturb the thermodynamical equilibrium sothat the ions migrate a distance x from their initial position toward the electrodeof opposite charge due to exerted electric forces on them as the charge carriers.Hence, an electrical mobility generates in the solution. Consequently, thedistance traveled by ions to the opposite charged electrode (Figure 3.15) is [5]where = Velocity of cations (cm/s)= Velocity of anions (cm/s)= Infinitesimal change of time (s)The number of ions that travel distance is
- 106 CHAPTER 3. KINETICS OF ACTIVATION POLARIZATIONwhere L = Distance between electrodes (Figure 3.15).Recall that electrical conduction is a mass transport phenomenon, in whichelectrons and ions carry the electric charge due to their particular mobilitywithin the electrically charged system. Hence, the charge (Q) that passesthrough the cross-section of the electrolyte solution (conductor) at time dt isrelated to the rate of flow of charge referred to as the current (I). It should bementioned that the electrons carry the current through the wires and electrodes,while the ions carry the current through the solution.This phenomenon implies that electrochemical reactions occur at the electrode-solution interface by transferring electrons from or to the electrode. For instance,if occurs, this means that one mole of is deposited onthe electrode surface while 2 moles of electrons flow through the circuit. Thissituation resembles an electrolysis process in which the cation valence iselectrons. Nevertheless, if the current is kept constant, the charge (q) that flowsthrough the circuit isThe total charge crossing a plane parallel to the electrodes in time dt [5]
- 3.8. CHARACTERIZATION OF ELECTROLYTES 107where = Electron charge =In addition, the current I and density areCombining eq. (3.80) and (3.82) yieldswhere V = AL = Volume of the solutionThe concentration (activity) of ions isCombining eqs. (3.10a), (3.76), (3.84) and (3.83) yieldsThe total current density becomes as in electrolysis. Hence,The ionic velocity for migration toward the electrode is small when com-pared with the random velocity based on the translational kinetic energy inthe absence of an electrical field [5]. This is mathematically shown belowFromeqs. (3.85) and (3.87),
- 108 CHAPTER 3. KINETICS OF ACTIVATION POLARIZATIONwhere = Mass of cations (species).In addition, electroneutrality is achieved when the rate of charge for cationsand anions balance and this is represented by However,the “quality ”of the electrolyte to act as an aqueous electrical conductor can becharacterized by its conductivity parameter For a one-dimensional analysis,iswhere = Conductivity= Resistivity (ohm .cm)= Electrical force gradient (V/cm)= Electrical potential at a point in the electrolyte solution (V)Furthermore, the effectiveness of ion migration can be characterized by theionic mobility in the solution when an electrical force field acts on the ions.This implies that the ionic mobility is related to the electrolyte conductivity.This can be assessed by substituting eq. (3.86) into (3.89)since the ionic or electrical mobility is defined aswhich has units of Normally, an electro-chemical process is analyzed using a particular metal ion in solution. As-suming that this is the case, eq. (3.91) can be treated in a general form. Hence,Then, and become
- or diffusivity of the metal cation as follows. Multiply both sides of eq.(3.94) by the Boltzmann constant and the absolute temperature T so thatNotice that is the Nernst-Einstein diffusion coefficient D, which is therate of swept area of cations [45]. Hence, the Nernst-Einstein equation isandThe subject of diffusion is well documented [37-45] and it is a manifestation ofcontinues atom or ion motion at random from position to a neighboring positionin the atomic structure of solids (S), liquids (L), and gases (G). Thus, thediffusivityis related tothe atomicjumpfrequency andjump distance. However,at a constant or the same temperature and diffusion in liquids differfrom diffusion in solids since the geometry of atomic arrangement in liquids isnot complete understood.In addition, electrolytes and n-type semiconductors conduct current by trans-port of ions and electron, respectively. Both ions and electrons are the chargecarriers for both sources. With regard to an electrolyte under the influence ofan electrical field, it can be expected that ions drift through the bulk aqueousmedium at a lower velocity than the electron velocity. However, the nature ofthe ions and their concentration influence both electrolyte conductivity andionicmobility as predicted by eqs. (3.93) or (3.94). If a relatively low steadypotential (voltage) is applied to electrodes, virtually current ceases toflowafterthe electrical double-layer capacitor is positively charged on the negativeelectrode surface and negatively charged on the opposite side at a distancefrom the electrode surface. The charged double-layer acts as an electrical capac-itor, which breaks down as the applied potential is increased beyond a criticalpotential for current flow to resume motion across the electrode-electrolyte in-terface. In this case, metal oxidation occurs at the positive electrode, whilereduction occurs at the negative electrode. Consequently, current flow causesenergy dissipation as heat in the electrolyte since the ions must overcome fric-tional forces during their motion through the medium [42].3.9 ELECTROLYTE CONDUCTIVITYThe influence of an electrical field on an electrolyte can also be characterized bymeasurements of the electrolyte electrical conductivity. In fact, electrolytes con-duct current by the bulk ionic mass transport and charge carrier across the ionic3.9. ELECTROLYTE CONDUCTIVITY 109From this crude approximation, one can determine the diffusion coefficient
- 110 CHAPTER 3. KINETICS OF ACTIVATION POLARIZATIONdouble-layer at the electrode surface. Consequently, in eq. (3.96) stronglydepends on the ionic concentration, temperature, and ionic mobilities. The ap-plication of an external potential along with an alternating current (AC) modeof frequency f causes current flow through the bulk electrolyte and charges theionic double-layer (Figure 2.7) as a capacitor. If current flows, then dissipationof electrical energy arises as heat in the bulk electrolyte and electrical energyis stored in the double layer capacitor. The dissipation of energy is attributedto the frictional forces during ionic mobility caused by the inner potentialThus, is the driving force for Faradaic processes (e.g. reduction and oxidationreactions) and electrolyte Ohmic resistance [42].The Wheatstone bridge shown in Figure 3.16 can be used to determine theelectrolyte resistance This is a classical technique reviewed by Braunstein-Robbins [42] who provided clear details on the current topic. Moreover, onlyone Wheatstone bridge case is briefly described hereafter.The expression given by eq. (3.89) is redefined as [43]where = Cell constantL = Distance between electrodes (cm)= Cross-sectional area of the electrolytic conducting pathAccording to Braunstein-Robbins [42], the Kholrausch method [43] can beused for evaluating In this method, the electrodes are electrolytically coatedwith colloidal platinum black in order to
- 3.9. ELECTROLYTE CONDUCTIVITY 111increase the electrode surface areareduce the polarization resistance that may develop andadsorb any gases produced during the cycle of the alternating current.On the other hand, AC is used in order to avoid changes of electrolyteresistance due to changes in concentration of the electrolyte and buildup ofelectrolysis products at the electrode surfaces [5]. Subsequently, ismeasuredat potential frequency (f) by adjusting the resistance so that the currentand potential are in-phase, which require a variable external conductanceAlso included in the Wheatstone bridge is the double-layer capacitor (C). Let’suse two different balance conditions.1) If the capacitance and C are excluded, then for a pure resistancecase the potential across points is and the potential balanceaccording to Ohm’s law isEliminating from eqs. (a) and (b) yieldsThen, eq. (3.99) becomes2) If the capacitance and C are included, then the circuit is not a pureresistance case and the potential drop across points is defined in termsofimpedance. Hence,This implies that and Insertingand into eq. (3.56) givesInserting eq. (3.103) into eq. (3.53) yields
- For an AC case with eq. (3.99) becomesThe potential expression given by eq. (3.104) can also be derive using com-plex function [42]. Hence,The charge (q) stored in the double-layer capacitor is related to thepotential drop across the capacitor as indicated belowCombining eqs. (3.109), (3.110) and (3.81) yieldsNow, using the complex functions defined by eqs. (3.107) and (3.108) on(3.111) givesThus,Letting andyields the applied potential112 CHAPTER 3. KINETICS OF ACTIVATION POLARIZATION
- 3.10. SUMMARY 1133.10 SUMMARYIn determining the rate of corrosion of a metal M, one needs to know the ki-netic parameters prior to computing it. Thus, the current density functionallows the evaluation of the corrosion behavior under acti-vation polarization at steady-state conditions. In order for polarization to occuron a metal surface, an overpotential must develop in the electrochemicalsystem and it is defined by the Tafel equation. Three electrochemical meth-ods were described for determining For instance, the linear polarizationmethod is applied at a small potential range of from thevalue. This method provides result for and On the otherhand, the extrapolation method generates anodic and cathodic curves near thecorrosion potential. These curves normally a small part of linearization fromwhich the Tafel slopes are determined and extrapolation of the linear lines con-verge at where is defined. The third method deals with impedancespectroscopy measurements (ISM). It is based on a transient current response toa potential excitation. This method allows the determination of the impedanceas a measurement of the polarization resistance and generates im-pedance data for modeling a corrosion process based on an electrochemical cir-cuit containing resistances and capacitors. This impedance technique is basedon AC circuit theory. The output of the impedance technique is a Nyquist plotfor charge-transfer or Nyquist-Warburg plot for diffusion control.Finally, mathematical models based on diffusion describe the generation ofcurrent density in a electrolyte solution in terms ofionic mobility and conductivecapacity of the electrolyte. Hence, the Nernst-Einstein equation for diffusivitywas determined.3.11 PROBLEMS/QUESTIONS3.1 What are the three conditions for galvanic corrosion to occur?3.2 If the state of equilibrium of an electrochemical cell is disturbed by anapplied current density then no longer holds. Let be acathodic current density and the slope of the corresponding polarization curvebe which increases approaching the Tafel constant Determinea) the value of when and and b) the valueof when and [Solutions: a)and b)3.3 According to the Stockholm Convention Cellthe corrosion potential of iron (Fe) is at and 25°C in adeaerated (no oxygen is involved) acid solution. Calculate a) the corrosion ratein when
- b) the Tafel anodic slope and c) draw the kinetic diagram E vs.[Solutions: a) b)3.4 Let the following anodic and cathodic reactions be, respectivelywhere and a) Construct the cor-responding kinetic diagram and b) determine both and from the diagramand from the definition of overpotential equations. [Solutions: b)and3.5 A steel tank is hot dipped in a deaerated acid solution ofmolality zinc chloride so that a 0.15-mm zinc coating is de-posited on the steel surface. This process produces a galvanized steel tank. Cal-culate the time it takes for the zinc coating to corrode completely at aData:[Solution: years].3.6 Calculate the activity and the corrosion rate of iron (Fe) immersed inan aerated aqueous solution of The dissociation constant for ferroushydroxide, is Given data:[Solution:3.7 Plot the anodic data given below and determine the polarization re-sistance and the anodic Tafel slope for a metal M. Useand[Solution: and3.8 Why does a pearlitic steel corrode rapidly in an acidic solution?3.9 Why will the tip and the head of an iron nail behave as anodes relativeto the shank? See Figure 1.10a.and114 CHAPTER 3. KINETICS OF ACTIVATION POLARIZATION
- 3.11. PROBLEMS/QUESTIONS 1153.10 It is known that the standard electrode potential (E°) for pure crys-talline zinc is –0.763 V. Will this value change by cold working and impurities?Explain.3.11 An electrolyte contains a very low activity of silvercations and an unknown concentration of copper cations. If the cellpotential difference between the copper anode and the silver cathode is –0.04V, determine a) which cation will be reduced (electroplated) on the cathodeand b) the concentration of in at 40°C. Neglect the effects of otherions that might react with silver. [Solution: a) will be reduced and b)3.12 Suppose that a cold worked copper electrode has 8,000 J/mol storedenergy and it dissolves in an aqueous electrolyte. Calculate the overpotential.3.13 What is the significant differences between the overpotential andthe Ohmic potential (E)?3.14 If a sheet of zinc is placed in hydrochloric acid (HCl), goesinto solution. Why?3.15 Calculate the equilibrium constant at 25°C for the electrochemical cellshown in Figure 2.4. [ Solution:3.16 Show that where the local potential E canbe defined by the Nernst equation.3.17 If an electrochemical cell operates at 10 amps, 25°C, and 101 kPa for30 minutes, calculate a) the number of moles and b) the weight of copper wouldbe produced. [Solution: a) N = 0.093 moles and b) W = 5.93 grams].3.18 a) Derive the Arrhenius equation from the general definition of theactivation energy of any rate reaction process and determine the Arrheniusconstants if and b) Plotvs.3.19 Plot the given conductivity data vs. the aqueous concen-tration at 25°C and 1 atm. (The data was taken from Ref. [5]). Conduct anonlinear regression analysis on these data and explain the resultant curve.
- 3.20 An electrochemical cell operates at a small overpotential and the cor-roding metal is exposed to a ion-containing electrolyte. Use the given datain order to determine a) the corroding metal by calculating the atomic weightand determining its anodic reaction. Assume that there is a linear relation-ship between the current density and the overpotential. b) The activity of thecorroding metal if c) the free energy change Will the reac-tion you have chosen occur?, d) the ionic velocity of the corroding metal. As acrude approximation, neglect the ionic velocity of other ions in solution, e) Thein the electrolyte. [Solution: b) d)3.21 If an electrochemical copper reduction process is carried out at 5amperes. for 20 minutes, determine a) the electric charge (amount of coulombsof electricity), b) the number of electrons if there areelectron/C, c)the number of moles, d) Faraday’s weight reducedon a cathode, and the reduction rate (production rate in Chapter 7). Data:and T = 35°C. [Solutions: a) Q = 6,000 C, b)electrons, c) N = 0.0311 moles, d) W = 1.98 g, and e)3.22 Calculate the overpotential that causes hydrogen evolution on a flatplatinum electrode surface immersed in an acid solution, when the appliedcathodic and exchange current densities are andrespectively. Assume a symmetry factor of 0.50 at room temperature (25°C).[Solution:116 CHAPTER 3. KINETICS OF ACTIVATION POLARIZATIONionic mobility and f) electrolyte conductivity neglecting other ions present
- 3.11. PROBLEMS/QUESTIONS 1173.23 Consider a discharge (chemical desorption) mechanism as the ratedetermining for at 25°C in a nickel battery. Calculate thecathodic Tafel slope per decade if the symmetry factor is 0.50, the exchangecurrent density is constant, and the cathodic overpotential is [Solution:3.24 Plot the normalized current profile as a function of both symmetryfactor and overpotential; that is, when the oxidation stateis defined is and and 0.75 at room temperature (25°C).Explain the polarization behavior very succinctly.3.25 Calculate the number of moles and mass of a) the battery zinccasing and b) the manganese dioxide in the electrolyte if the batteryhas a stored energy of and a power of 3 Watts. Calculate c) the timeit takes to consume the stored energy if the battery operates at a current of 2A and d) the potential (voltage). The thickness of the cell casing isand other dimensions are indicated below. The discharging reaction is[Solution: a) and 0.62 moles, b) 0.37 moles and c) and1.5 V]3.26 A plate of pure nickel oxidizes in an electrochemical cell con-taining an acid solution at 25°C. The total surface area of the nickel plate isIf electrons per second are relieved on the plate surface, thencalculate a) the corrosion rate in and b) the mass of nickel being lost ina year. [Solution: a) and b)3.27 Use the data listed in Table 3.3 to perform a least squares analysisand subsequently, determine the polarization proportionality constant Letthe atomic weight and the density of the steel beand respectively. [Solution:
- 3.28 Equal amounts of and are dissolved with water tomake up an electrolyte. Hypothetically, the ion velocities and concentrationsareIf the current density is calculate the velocity of the nickel ions[Solution: 0.20 cm/s].3.29 An electrochemical cell operates at 10 A, andDetermine a) the electrolyte resistance b) the potential when theexternal resistance and the capacitance are andat 30°C and c) the electrolyteconductivity The distance between electrodesis L = 15 cm and the effective electrode surfaceis [Solution: a)b) and c)3.30 Determine and analyze the impedance profile by varying the angularfrequency for fixed and3.31 Assume that an electrolytic cell is used for recovering nickel from asolution containing of at 35°C. The nickel ionic mobilityand the electric-field strength are and[Taken from reference 5], respectively, calculate a) the ionicvelocity b) thesolution electric conductivity and the electric resistivity [Solution:a) b) and c)3.32 It is known that current flows when there exists a gradient of electricpotential within an electric conductor, such as an electrolyte. Considera current-carrying homogeneous conductor with constant cross-sectional areaso that the electric-field strength is constant at every point in theconductor. Derive an expression for the current as a function of the gradientof electric potential. In this particular problem stands for direction as wellas length of the electric conductor. Start with the following current densitydefinition where is the electric conductivity3.12 REFERENCES[1] M.G. Fontana, “CorrosionEngineering,”third edition, McGraw-Hill BookCompany, NewYork, (1986).[2] T.N. Andersen and H. Eyring, “Principles of Electrode Kinetics” inPhysical Chemistry: An Advanced Treatise, Vol. IXA/Electrochemistry, Editedby Henry Eyring, Academic Press, Inc., (1970).118 CHAPTER 3. KINETICS OF ACTIVATION POLARIZATION
- 3.12. REFERENCES 119[3] D.W. Shoesmith, “Kinetics ofAqueous Corrosion,” in Corrosion, ASMHandbook, Vol. 13, American Society for Metals, Ninth edition, (1987).[4] D.A. Jones, “Principles and Prevention of Corrosion,” Macmillan Pub-lishing Company, New York, (1992).[5] I.N. Levine, “Physical Chemistry” McGraw-Hill Book Company, NewYork, (1978) 454-459, 498-500.[6] A.J. Bard and L.R. Faulkner, “Electrochemical Methods,” John Wiley& Sons, New York, (1980) 316.[7] L.L. Shreir, “Outline of Electrochemistry,” in Corrosion, Vol. 2, Corro-sion Control, Edited by L.L. Shreir, R.A. Jarman, and G.T. Burstein, Butterworth-Heinemann, Boston, (1994).[8] U.R. Evans, J. Franklin Institute, 208 (52) (1929).[9] U.R. Evans, “The Corrosion and Oxidation of Metals,” Arnold, London,(1961).[10] M. Stern, J. Electrochem. Soc., 104 (1957) 56.[11] M. Stern, J. Corrosion, 13 (1957) 755.[12] L.L. Shreir, “Corrosion in Aqueous Solutions” in Corrosion, , Vol. 1,Metal/Environment Reactions, Edited by L.L. Shreir, R.A. Jarman, and G.T.Burstein, Butterworth-Heinemann, Boston, (1994).[13] J.R. Scully, “Electrochemical Methods of Corrosion Testing,” in Corro-sion, Vol. 13, Laboratory Testing, ninth edition, ASM Inter. (1987) 213.[14] H.P. Hack, “Evaluation of Galvanic Corrosion,” in Corrosion, Vol. 13,Ninth edition, ASM Inter., (1987) 236.[15] J.R. Maloy, J. Chem. Educ., 60 (1983) 285.[16] J. Wang, “AnalyticalElectrochemistry,” Second edition, Wiley-VCH,Inc., (2000) 4-7.[17] J.W. Evans and L.C. De Jonghe, “The Production of Inorganic Mate-rials” Macmillan Publishing Company, New York, (1991) 149.[18] T. Erdey-Cruz, “Kinetics of Electrode Processes” Wiley-Interscience,New York, (1972) 442.[19] D.D. McDonald, J. Electrochem. Soc., 125 (1978) 1443.[20] A.C. Makrides, Corrosion, Vol. 18, (Sept. 1962) 338.[21] A.C. Makrides, J. Electrochem. Soc., 107 (1960) 869.[22] F. Mansfeld, Corrosion, Vol. 36, 5 (1981) 301-307.[23] F. Mansfeld, Corrosion, Vol. 38, 11 (1982) 570.[24] J.R. Scully, Corrosion, Vol. 56, 2 (200) 1999.[25] J.H. Wang, F.I. Wei, and H.C. Shih, Corrosion, Vol. 52, 8 (1996) 600.[26] E. Khamis, M.A. Ameer, N.M. Al-Andis, and G. Al-Senani. Corrosion,Vol. 56, 2 (2000) 127.[27] P. Piereon, K.P. Bethune, W.H. Hartt, and P. Anathakrishnan, Corro-sion, Vol. 56, 4 (2000) 350.[28] D.W. Law, S.G. Millard, and J.H. Bungey, Corrosion, Vol. 56, 1 (2000)48.[29] D.D. McDonald and M.H. McKubre, in Modern Aspects of Electro-chemistry, Edited by J. O’M. Bockris, B.E. Conway and R.E.White, Vol. 14,Plenum Press, New York, (1982) 61.
- [30] K. Hladky, L.M. Callow, and J.L. Dawson, Br. Corrosion Journal, Vol.15, 1 (1980) 20.[31] O.C. Ho, D. Raistrick, and R.A. Huggins, Electrochem. Acta, 127(1980) 343.[32] D.R. Franceschetti and J.R. McDonald, Electrochem. Acta, 129 (1982)1754.[33] M.W. Kendig, E.T. Allen, and F. Mansfeld, J. Electrochem. Soc., 131(1984) 935.[34] R. Delevie and L. Pospisil, J. Electroanal. Chem., 22 (1969) 277.[35] L. Nyikos and T. Pajkossy, Electrochem. Acta, 35 (1990) 1567.[36] K.S. Cole and R.H. Cole, J. Chem. Phys. 9 ( 1941) 341.[37] P.G. Shewmon, “Diffusion in Solids,” McGraw-Hill, New York, (1963).[38] R.J. Weiss, “Physics of Materials,” Hemisphere Publishing Corp., NewYork, (1990) 360-362.[39] A.G. Guy and J.J. Hren, “Physical Metallurgy” Third edition, Addison-Wesley Publishing Company, Reading, Massachusetts, (1974) 367-399.[40] C.A. Wert and R.M. Thompson, “Physics of Solids,” Second edition,McGraw-Hill Book Company, New York, (1970) 54-73.[41] J. Crank, “The Mathematics of Diffusion,” Second edition,, OxfordUniversity Press, New York, (1990).[42] J. Braunstein and G.D. Robbins, J. Chem. Edu., Vol. 48, 1 (1971)52-59.[43] F. Kohlrausch, Weid. Ann., 60 (1897) 315.[44] B. Wu and R.E. White, “Modeling of a Nickel-Hydrogen Cell: PhaseReactions in the Nickel Active Material,” J. Electrochemical Soc., Vol. 148, No.6 (June 2001) A595-A609.[45] G.H. Geiger and D.R. Poirier, “Transport Phenomena in Metallurgy”Addison-Wesley Publishing Company, Reading, Massachusetts, (1973) 434, 443,449-451.[46] M. Pourbaix, “Lectures of Electrochemical Corrosion,” Plenum Press,New York, (1973) 239-252.120 CHAPTER 3. KINETICS OF ACTIVATION POLARIZATION

Full NameComment goes here.